Low-temperature epitaxial growth of thin metal
James W. Evans
Iowa State University
D. E. Sanders
Iowa State University
Patricia A. Thiel
Iowa State University
Andrew E. DePristo
Iowa State University
Follow this and additional works at:
Part of the
Biological and Chemical Physics Commons
, and the
Physical Chemistry Commons
The complete bibliographic information for this item can be found at
. For information on how to cite this item, please visit
This Article is brought to you for free and open access by the Chemistry at Iowa State University Digital Repository. It has been accepted for inclusion in Chemistry Publications by an authorized administrator of Iowa State University Digital Repository. For more information, please contact
Low-temperature epitaxial growth of thin metal films
We present a different mechanism to explain the occurrence of long-lived oscillations in diffraction spot
intensities during epitaxial growth of metal films on fcc (100) substrates at low temperature. Rather than rely
on the common picture of cyclical nucleation and growth to produce the oscillations, the model invokes
‘‘downward funneling’’ deposition dynamics to fourfold-hollow adsorption sites.
Ames Laboratory, Physics and Astronomy
Biological and Chemical Physics | Physical Chemistry
This article is from
Physical Review B
41, no. 8 (1990): 5410–5413, doi:
PHYSICAL REVIE% B yOLUME 41,NUMBER 8
15 MARCH 1990-I
The Rapid Communications section is intended for the accelerated publication
ofimportant new results Si.nce manuscripts submitted to this section are given priority treatment both in the editorial office and in production, authors should explain in their submittal letter why the workjusttftes this special handling A Rapid Communication should be no longer than 3H printed pages and must be accompanied by an abstract Pa.ge proofs are sent to authors, but, because
ofthe accelerated schedule, publication isnot delayed
ofcorrections unless requested by the author or noted by the editor
P.A. Thiel, and Andrew
ofPhysics and Chemistry, and Ames Laboratory, iowa State University, Ames, iowa 500ll
(Received 5October 1989)
We present a different mechanism to explain the occurrence of long-lived oscillations in diffraction spot intensities during epitaxial growth of metal films on fcc(100) substrates at low temperature. Rather than rely on the common picture of cyclical nucleation and growth to pro-duce the oscillations, the model invokes "downward funneling" deposition dynamics to
fourfold-hollow adsorption sites.
There have been many experimental observations
long-lived oscillations in reflection-high-energy electron diffraction
(RHEED)during epitaxial growth
ofsemicon-ductor and metal films. ' Traditionally, such oscilla-tions have been associated with layer-by-layer growth, in-volving cyclical nucleation, growth, and coalescence of
is-lands in each layer, made possible by thermal diffusion.
However, long-lived oscillations have been reported re-cently during epitaxial growth at temperatures solow that thermally activated surface diffusion is thought to be
iThis prompted the proposal2 that the nucleation and growth picture essentially still applies with
"transient diffusion" or ballistic motion
ofthe adsorbate replacing thermal diff'usion. This transient diffusion is
en-visioned to result from the need to dissipate the energy released upon formation
ofthe atom-surface bond. This
event isexothermic by up to 3 eV
(69kcal/mol) for metal-lic systems. '
In this paper, we demonstrate that neither traditional nucleation and growth nor transient diffusion are
neces-sary to obtain long-lived diffraction intensity oscillations
in low-temperature epitaxial growth on
sub-strates. The term transient diffusion is used here
speci-fically torefer to motion from one fourfold-hollow adsorp-tion site to another. Such motion necessarily involves a component perpendicular to the direction of vertical
im-pingement on the
(100)face. Instead we show that these oscillations can result primarily from a "downward fun-neling" prescription
ofthe deposition dynamics incor-porating the physically reasonable fourfold-hollow adsorp-tion site requirement. Such downward funneling might
correspond to channeling down the
micro-pyramids which develop during film growth (after
im-pingement at 45 in these
faces).We conclude by
presenting independent molecular-dynamics
ofthe deposition dynamics
ofindividual atoms using
corrected effective medium
(CEM)based interaction po-tentials. These show conclusively that adsorption on
fcc(100)metals leads irreversibly to binding at a
fourfold-hollow site without transient mobility. These
MD studies also generally support the downward funnel-ing picture.
There are several previous studies pertinent to
low-temperature film growth. One very simple and well-known model involves random, immobile deposition
particles onto the tops ofcolumns growing from the
ofa simple-cubic crystal. Here the column heights satisfy a Poisson distribution with standard deviation
(in-terface width) equal to
eis the mean cover-age in monolayers. Since diffraction from this growing film does not produce oscillations, the model fails to de-scribe the above-mentioned experimental behavior. (This
simple model probably spawned the widespread belief that some sort
ofmobility isessential to achieve oscillations.
ln contrast to this model, MD studies
ofdeposition on a
fcc(111)substrate using simple Lennard-Jones potential indicated significant transient diffusion, at least, in the
first layer at
0 K.This facilitates ordering, as re-flected by a first layer saturation coverage
compared with 76% for random immobile deposition. (Filling is incomplete due to domain boundaries, which
cannot develop in the models we consider.
MD simulations, described below, indicate that this be-havior is due to having only one movable substrate layer.
The degree ofmobility is greatly reduced with three
mov-able layers. Finally, we note that simple Monte Carlo
(MC)modeling shows that transient diffusion leads to smooth films, and the appearance
Our aim here is to develop models for fcc epitaxial
growth via deposition at fourfold-hollow sites starting from a
(100)substrate. We first categorize all fcclattice
LOW-TEMPERATURE EPITAXIAL GROWTH OFTHIN METAL FILMS
I&I I I I I I
I I I I
I I I I I I I I I I I I I I
l 1 lI I I I II I I l II I I I II I I I II I I I II I
I I I I I I I I II I I I I I s I & I I
(a)RANDOM DEPOSITION (b) DOWNWARD FUNNELING
FIG.1.Schematic ofrandom immobile deposition (Ref. 7)vs
downward funneling deposition dynamics.
FIG.2. Capture areas forcontinuous downward funneling.
sites where adsorption has or potentially can occur as
ei-ther filled, empty complete, or empty incomplete
adsorp-tion sites. Complete adsorption sites have a cluster
k 4 supporting atoms in the layer beneath, whereas
in-complete adsorption sites have 1
exact analytic solution was obtained for the model where
the adsorption probabilities are nonzero (and equal) only
at complete adsorption sites. This simplistic choice
adsorption probabilities produces nontrivial film growth which is initially quite layer-by-layer-like, but becomes
less and less so as deposition progresses. Associated diffracted intensity oscillations effectively die out by
3.This model mimics the experimental
LEEDoscil-lations, but not the sticking coefficient behavior observed for Pt/Pd(100) at 80
K.' In contrast,
RHEEDoscilla-tions in other metallic systems are long lived, which rules
out the applicability of this simple model. However, we show that aslight tnodification
ofthe deposition dynamics
in this model produces surprisingly long-lived oscillations
which are in qualitative agreement with the
This modified model incorporates downward funneling to complete adsorption sites
ofall impinging atoms at
0K (see Fig.
1).Here it is assumed that these atoms
impinge vertically with acontinuum
0K process is deterministic, there isa unique adsorption site associated with each
e.,for any film configuration the
Xispace can be parti-tioned into "capture zones" for the various complete ad-sorption sites. Thus, we simulate the deposition process
by allowing complete adsorption sites to fill at rates pro-portional to their associated capture areas (rather than
with equal rates as above and in
Consider 6rst the funneling-off layer
jatoms to com-plete adsorption sites supported by layer
funneling off first layer atoms to adsorption sites on the
substrate), and assume that the shape ofthe capture zone
is influenced only by atoms diagonally or laterally
adja-cent to the adsorption site.
Ifthere are no such adjacent
atoms, then by symmetry, the capture zone is the square
shown in Fig.
the capture zones for adsorption sites with one diagonal or one latterally adjacent atom. Clearly their areas AD and AL, respectively, must satisfy 4AD+4AL,
9.The capture zone area A~L for an adsorption site with the diagonally
and laterally adjacent atoms shown in Fig.
4A~+2AL+4ADL 12. Continuing in this way, one can
express the capture zone area for an adsorption site with any number
ofdiagonally and laterally adjacent atoms in
ofone free parameter, AD=
1+BD,say. We note
FIG. 3. Partition ofXll space for discretized downward fun-neling.
that the need to catalog capture zone areas for funneling
offhigher layer atoms tolower layer adsorption sites con-stitutes a major complication in this model since somany
configurations inust be considered.
It is thus convenient to introduce a discretized version
ofthe downward funneling model which is simpler to im-plement. We utilize the concept ofcomplete
3)adsorption sites as described above. One starts by partitioning the
Xispace as shown
3.Any atom impinging on a large square region is assigned permanently tothe corresponding k 4complete adsorption site. Any atom impinging on an L shaped, rec-tangular or small square region is assigned initially to the corresponding k 3, 2,1 incomplete adsorption site, re-spectively. (These assignments are simply achieved by filling adsorption sites at rate
k/4. )Then immediately this atom is moved progressively downward to (adjacent)
lower adsorption sites until a complete one isfound. More specifically, if k 3 the downward move is uniquely
Ifk 2, there are two adjacent lower adsorp-tion sites and one is chosen randomly.
Ifk 1, the atom
moves to a diagonally adjacent lower site with probability 4b, or to one
ofthe two laterally adjacent lower sites with
—46)/2 (see Fig.
For these models, let
8Jdenote the coverage (in mono-layers)
0corresponds to the top sub-strate layer, so
—8~+~ reflects the net number ofexposed atoms in layer
j.We consider the
(i)The interface width W satisfying W2
(the total coverage). '
(ii)The step density which is simply taken as the
empty-filled sites in the
destructive-5412 EVANS, SANDERS, THIEL,AND DEPRISTQ 0.0
ro«««I C a b 0%$%looouoo%% OISIN«««IO«IS«OI O.S-Q
~ y+0~ ~oQI+~ o«e
MwegyggtM wQ~~ ~ggf—
FIG.4. Interface width, step density, and Bragg intensity
be-havior for (a) random immobile deposition (Ref. 7), (b)
simplified continuous downward funneling, (c) discretized
downward funneling, and (d)one-hop transient mobility models.
)assuming equal scattering factors for substrate and film atoms.
of RHEEDintensity oscillations should be refiected in the behavior
Ia,and of the step density. Neglect
ofmultiple scattering rules out quantitative agreement with
Ia„however.Results below are obtained from MC simulation. Since the models considered here generate only very short-range spatial correlations (for
ca. 30MC trials on a 100X100substrate are
sufficient to obtain essentially exact statistics.
Figure 4 contrasts the behavior
ofthese quantities for random immobile deposition at fourfold-hollow sites
7),the discretized funneling model with b
ofthe continuum funneling model. The latter considers only layer
jatoms when calculating
cap-ture areas for adsorption sites supported by layer
atoms, and sets bD
6.This parameter choice
corre-sponds to a hard-sphere potential where impinging atoms make contact with film atoms and then slide "downhill" to
an adsorption site. Note that for layer-by-layer growth, W
these functions repeat periodically for higher
e.For ran-dom-4edeposition on top
One finds persistent long-lived
la,oscillations in the funneling models, in marked contrast to the simple ran-dom immobile deposition model
the full continuum model are undoubtedly larger than in
the simplified version shown. Clearly these models in-clude no propensity for island formation in the usual
sense, their spatial pair correlations always remaining short ranged. However, the observed oscillations indicate the (rapid) development
wherein the film structure roughly repeats itself with
x+1).This behavior is clearly refiected in
the slowly increasing surface width. Growth isnot strictly layer-by-layer, but at most a couple
significant partial coverage at any one time.
ofthe funneling models reveals that the funneling dynamics enhance short-range clustering
(i.e.,increase the NN spatial pair correlations) relative to
random deposition. '3 Thus funneling produces more ad-sorption sites in the upper layer, which alone would make growth less layer-by-layer-like. However, funneling also boosts the filling rate for lower layers relative to random deposition. The latter eA'ect dominates in this competi-tion, producing quasi-steady-state growth. (In contrast, for an analogous 1D bridge-site deposition model, these competing effects roughly cancel.
We assert below that transient diffusion is absent at
0Kin metal-on-metal systems. However, it isstill
in-structive to compare the behavior
ofthe above funneling models with that for models incorporating very short-range transient mobility. Thus we modify the model
Ref.7 for random immobile deposition at fourfold-hollow sites by allowing atoms to make one hop to a randomly
chosen empty neighboring site immediately after deposi-tion.
Ifthat site is complete
4)the atom remains there. Otherwise it tumbles downhill, as in the discrete
funneling model. The
Ia,oscillations are even larger than for the funneling models, and oscillations are visible in the step density and interface width (see Fig.
4).In another modification
ofthe model of
Ref.7, atoms adsorbing at
complete fourfold-hollow sites "knock
supporting atoms toan adjacent empty site
and then take its place. The dislodged atom stays at the empty site if complete
4),or otherwise tumbles
downhill to a complete adsorption site. Oscillations in
measured quantities here are larger than in the above one-hop (oreven an extended two-hop) transient mobility model. Clearly, transient mobility or knockout phenome-na enhance the layer-by-layer character ofgrowth. How-ever, our main point in this paper isthat these phenomena
are not necessary to achieve the long-lived oscillations in
Ia,which are usually taken as experimental confirmation
Finally we performed MD studies
ofindividual atoms, designed to check the validity
ofthe above ideas. Several systems were considered, in-cluding Cu/Cu(100),
Pt/Pd(100),and Cu/Ag(100) using
sophisticated interaction potentials obtained from the
corrected effective medium theory. These should be quite reliable for metallic systems. In contrast, Lennard-Jones
6)potentials used previouslys cannot accurately de-scribe the elastic constants, binding energy, and lattice
constant, simultaneously. In our simulations, one atom
&250 "target"substrate atoms in three
movable layers with Langevin coupling to the rest
ofthe bulk. ' The analysis reveals that transient motion does not occur at 80
K.Rather, the atom always settles into the fourfold-hollow site on which itimpinges (see Fig.
This result is insensitive tothe initial kinetic energy
impinging atom at least up to
-0.25 eV, since the near-surface kinetic energy is determined primarily by the
sup-LOW-TEMPERATURE EPITAXIAL GROWTH OFTHIN METAL FILMS 5413
FIG.5. Deposition dynamics for0.25-eV Cuimpinging
verti-cally on aCu(100)surface held at 80 K. Only asmall subset of
the moving substrate atoms is shown. The time increment (from left to right) is0.20ps.
grate even a single lattice constant away from the initial
impingement site. Thus, the MD simulations using
potentials, and the earlier
FIMmeasurements both serve
to rule out the idea
oftransient mobility in metal-on-metal systems. Consequently, we conclude that the tradi-tional picture
ofmobility-mediated island nucleation and growth does not describe low-temperature epitaxial
ofthin metal films. However, an alternative mod-el incorporating downward funneling to physically reason-able fourfold-hollow adsorption sites is herein provided. This model can explain the long-lived oscillations observed
in the diH'racted intensities, and the associated quasi-steady-state growth.
port the funneling picture. Dynamics following
impinge-ment on larger inclines is more complicated, but these configurations are statistically rare. These studies also
in-dicate that the knockout mechanisms, described above, are typically inoperative.
Our MD results agree, in fact, with earlier field-ion-microscopy
(FIM)measurements, ' which showed that
tungsten atoms evaporated on a W tip at 80 Kdo not
mi-This work was supported by National Science
Founda-tion Grants No.
Cray Research Inc.,Camille and Henry Dreyfus Founda-tion,
S.),and the Ames Laboratory. Ames Laboratory is operated for the
Ener-gy by Iowa State University under Contract No.
W-7405-ENG-82. This work was supported by the Office
'Reflection High-Energy Electron Digraction and Reflection Imaging
ofSurfaces, edited by P. K.Larson and P.
(Plenum, New York, 1988).
2W. F.Egelhoff and
I.Jacob, Phys. Rev. Lett. 62, 921 (1989). Many references aregiven here which describe the traditional
nucleation and growth picture.
C.Koziol, G.Lilienkamp, and
E.Bauer, Appl. Phys. Lett. 51,
4J. D.Kress, M. D.Stave, and A. E.DePristo,
93, 1556(1989); T.
J.Racker and A.E.DePristo, Phys. Rev.
sF.Reif, Statistical and Thermal Physics (McGraw-Hill, New
M. Schneider, A.Rahman, and
I.K.Schuller, Phys. Rev. Lett.
7J. W.Evans, Phys. Rev. B 39, 5655
J.Phys. A 19,L441
sS.Clarke and D.D.Vvedensky, Phys. Rev.B37,6559(1988).
' D. K.Flynn,
J.W. Evans, and P.A. Thiel,
Tech-nol. A7, 2162
"M.Thomsen and A. Madhukar,
J.Cryst. Growth 80, 275
S.Lent and P.
I.Cohen, Surf. Sci. 139,121 (1984). '3J.W.Evans (unpublished).
'4A.E.DePristo and H.Metiu,